(2) 440. Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. samples were subjected to X-ray diffraction, scanning electron microscopy, particle size, impedance spectroscopy and linear sweep voltammetry analysis. 2. Experimental procedure 2.1. Synthesis of Mg0.5+x/2Si2-xAlx(PO4)3 samples For sample preparation, magnesium acetate tethrahydrate (C4H6MgO4∙4H2O), tetraethyl orthosilicate (SiC8H20O4), aluminum acetate (C6H9AlO6) and ammonium phosphate monobasic (H6NO4P) were used as the starting materials. Meanwhile citric acid (C6H8O7) was employed as the chelating agent. The molar ratio of Mg:Si:Al:P:O was determined based on the stoichiometric formula of Mg0.5+x/2Si2-xAlx(PO4)3 with x = 0.10, 0.15, 0.20 and 0.25. The starting materials were first dissolved separately in distilled water and then stirred for 1 h under magnetic stirring at a temperature of 30 °C. All of the solutions were mixed together and stirred in a reflux system at 70 °C for 24 h to form a homogeneous solution. The solution was taken out and then evaporated for at least 7 h under magnetic stirring at 80 °C. The resulting wet gel was dried in a vacuum oven at 150 °C for 24 h to remove water particles and organic resistance. The obtained powder was heated at 400 °C for 4 h to remove ammonium and acetate groups. The powders obtained were pressed using a Specac pellet press at 3 tons pressure to form pellets with mass, diameter, thickness, and density of 0.5 g, 13 mm, 2 mm and 1.88 g/cm−3, respectively. Eventually, the samples were later annealed at sintering temperatures of 800 °C for 4 h. 2.2. Characterization techniques The X-ray powder diffraction analysis was carried out using PANalytical-X’pert3 X-ray diffractometer with Cu-Kα radiation of wavelength of 1.5406 Å in 2θ range from 10° to 40°. Then, the monoclinic lattice parameters of the samples were calculated using the formula [8]:. 1 1 ⎛ h k sin β l 2hl cos β ⎞ = + + 2− d 2 sin 2 β ⎜⎝ a2 b2 c ac ⎟⎠ 2. 2. 2. 2. (1). and. d=. λ 2sin θ. (2). where d is the distance between crystal planes of (hkl), λ is the X-ray wavelength, θ is the diffraction angle of crystal plane, hkl is the crystal index, a, b and c are the lattice parameters and β is the angle between a and c. A Zeiss-Evo MA10 scanning electron microscope was used to conduct morphological analysis of the Mg0.5+x/2Si2-xAlx(PO4)3 powders. The particle size information of the ceramic samples was acquired using FRITSCH-Analysette 22 NanoTec laser particle sizer at room temperature. The density (ρ) was also calculated from the mass and sample dimensions using following equations [9,10],. ρ=. m π r 2t. (3). where m is the mass, r is the radius and t is the thickness of the pallet. Complex impedance parameters (i.e. impedance and phase angle parameters) were measured with a computercontrolled Solatron 1260 impedance analyzer. The samples were sandwiched between platinum electrodes which served as non-blocking electrodes in a frequency range from 0.1 to 106 Hz. The total conductivity, σt (bulk conductivity, σb + grain boundary conductivity, σgb) which represents the direct current (dc) conductivity in the ceramic sample was calculated using the equation:. 1 1 1 = + σ t σ b σ gb. (4). d d and σ gb = ARgb ARb In these equations, d is the sample thickness, A is the crosssectional area of the sample, Rb is the bulk resistance and Rgb is the grain boundary resistance. Ac conductivity has been evaluated from dielectric data in accordance with the relation: where σ b =. σ ac = ωε oε ′′ tan δ. (5). where εo is the permittivity of the free space (8.854 × 10−14 F cm−1), ω = 2π f , ε″ is the dielectric loss and tan δ is the loss tangent factor. The electrochemical stability of the studied samples was evaluated by LSV using Wonatech ZIVE MP2 multichannel electrochemical workstation. The samples were placed between two stainless steel blocking electrodes and a potential current of 0.5 V was applied in order to polarize them. The current was then monitored as a function of time until it reached a steady state condition. Magnesium transference number measurement was performed using Bruce and Vincent method in order to determine the actual type of charge carriers. The magnesium transference number (τMg2+) was calculated using the equation [10,11]:. τ Mg 2+ =. I ss ( ΔV − I o Ro ) I o ( ΔV − I ss Rss ). (6). where Io is initial current (t = 0), Iss is steady state current, Ro and Rss are the initial resistance of the passive layer (before polarization) and the resistance of the passive layer (after polarization) respectively and ΔV is applied voltage bias (ΔV = 0.27V). 3. Result and discussion Presented in Fig. 1 is the XRD spectra of Mg0.5+x/2Si2-xAlx(PO4)3 (x = 0.10, 0.15, 0.20 and 0.25) samples. All of the samples exhibit sharp diffraction peaks attributed only to Mg0.5+x/2Si2-xAlx(PO4)3 which proves that all compounds were pure. The XRD spectra of the samples were indexed to monoclinic structure with a space group of P121/c1. All of the Mg0.5+x/2Si2-xAlx(PO4)3 peaks are sharp and well defined, indicating that the samples are generally well crystallized. There are synchronizations between the result of lattice parameters, crystallite size, density and volume of the samples which increase with the increase of x as shown in Table 1. The.

(3) Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. 441. Fig. 1. X-ray diffractograms Mg0.5+x/2Si2-xAlx(PO4)3 samples.. increase of Mg-ion interstitial was found to affect the structures of the ceramic compounds. The increase in the unit cell volume is attributed to the larger atomic size of Al3+ than Si4+ and due to the existence of additional interstitial Mg2+ ion after successful partial substituted process in the samples. It is also shown that the density of all compounds have been decreasing after the sintering process. This is because of the thermal shrinkage process in sol-gel method [12]. Meanwhile, the increase in the crystallite size is due to the grain growth process on the samples [13,14]. SEM micrographs and particle size distributions of the Mg0.5+x/2Si2-xAlx(PO4)3 (x = 0.10, 0.15, 0.20 and 0.25) samples are displayed in Fig. 2 and Fig. 3 respectively. SEM micrographs show that the particle size increases from x = 0.10 to x = 0.25. Meanwhile, Fig. 3 clearly shows that the size of the particles in Mg0.5+x/2Si2-xAlx(PO4)3 samples increases with the increase of x. As the x increases, the average size of the particles in the Mg0.5+x/2Si2-xAlx(PO4)3 samples increases from 35.7 µm to 58.9 µm. The impedance plots of the Mg0.5+x/2Si2-xAlx(PO4)3 (x = 0.10, 0.15, 0.20 and 0.25) samples are shown in Fig. 4. The impedance plot for every sample consists of two overlapping semicircles with a titled spike at low frequency region. The high frequency semicircle is ascribed to bulk response with its. Table 1 Lattice parameters, unit cell volume, crystallite size and density of Mg0.5+x/2Si2-xAlx(PO4)3 samples. Samples. α(Å). b (Å). c (Å). V (Å3). Crystallite size (Å). Density (gcm−3). x = 0.10 x = 0.15 x = 0.20 x = 0.25. 6.707 6.720 6.733 6.740. 5.750 5.755 5.764 5.774. 12.433 12.456 12.501 12.524. 479.496 481.687 485.172 487.327. 86.299 115.100 115.100 138.099. 1.412 1.410 1.411 1.410. intercept at the x-axis attributed to bulk resistance, Rb, while the middle frequency semicircle is associated to grain boundary response with its intercept at the x-axis corresponding to grain boundary resistance, Rgb [15]. On the other hand, the spike that can be clearly seen at the low frequency region of the spectra indicates the effects of electrode polarization as a result of accumulation of ions between electrode and samples [16]. The complex impedance data obtained experimentally for the Mg0.5+x/2Si2-xAlx(PO4)3 (x = 0.10, 0.15, 0.20 and 0.25) samples at room temperature may be approximately denoted by the impedance of an equivalent circuit consisting of bulk resistance (Rb), grain boundary resistance (Rgb), bulk, Cb (CPE), grain boundary capacitance Cgb (CPE) and CPE blocking electrode as shown in Fig. 5. Table 2 lists direct current conductivity values of all Mg0.5+x/2Si2-xAlx(PO4)3 samples calculated using Eq. (3). The conductivity increases consistently from x = 0.10 to x = 0.25. The sample with x = 0.25 gives the highest bulk conductivity with value of 1.54 × 10−4 S cm−1 at ambient temperature which is an order of magnitude higher compared to that of the parent compound, Mg0.5Si2(PO4)3 as reported in reference [4]. This demonstrates that insertion of Al3+ slightly increases the conductivity of this compound by producing additional interstitial Mg2+ which increases the number and mobility of ions. Fig. 6 presents the graph of log σ(ac) versus log ω for the Mg0.5+x/2Si2-xAlx(PO4)3 (x = 0.10, 0.15, 0.20 and 0.25) samples. The plot can be divided into three regions; the low frequency, intermediate frequency and high frequency regions. The spectra exhibit a spike in low frequency region due to the polarization effects where the blocking of ions between the sample and electrode occurs. There is a plateau at the intermediate frequency region and extrapolating it to the y-axis gives the value of direct current conductivity, σdc [17,18]. In this region, the conductivity is frequency independent and the σdc values are found to be in good agreement with the values listed in Table 2..

(4) 442. Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. Fig. 2. Cross-sectional SEM micrographs of the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25.. Fig. 3. Particle size distribution of the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25..

(5) Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. 443. Fig. 4. Typical complex impedance plots of the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25.. Fig. 5. Equivalent circuit of Mg0.5+x/2Si2-xAlx(PO4)3 samples based on the impedance analysis of the samples at room temperature.. On the other hand, at high frequency region, the transition from direct current plateau to alternate current conductivity dispersion occurs. According Almond and co-workers [19], the ionic hopping ωp can be directly obtained from alternate current conductivity graph. The value of ionic hopping ωp can be obtained by extrapolating, at twice the value of direct current conductivity, from the vertical axis horizontally toward the graph and then extrapolating downwards vertical to the horizontal axis as shown in Fig. 6. Using the ωp value, the magnitude of the charge carrier concentration, K can be calculated using the equation as follows [20,21]:. K= Table 2 The σb, σgb and σt of Mg0.5+x/2Si2-xAlx(PO4)3 samples at ambient temperature. Sample. x. σb (S cm−1). σgb (S cm−1). σt (S cm−1). Mg0.5+x/2Si2-xAlx(PO4)3. 0.10 0.15 0.20 0.25. 1.27 × 10−5 2.94 × 10−5 2.52 × 10−5 1.54 × 10−4. 5.11 × 10−6 1.17 × 10−5 1.86 × 10−5 3.39 × 10−5. 3.65 × 10−6 8.37 × 10−6 1.07 × 10−5 2.78 × 10−5. σT ωp. K = ne 2 a2γ k −1. (7) (8). where e is electron charge, γ is correlation factor which is set equal to 1, and a is the jump distance between two adjacent sites for the ions to hop that is assumed to be 3 Å [22]. The density of mobile ions (Mg2+), n, can be determined using Eq. (8), and.

(6) 444. Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. Fig. 6. Alternate current conductivity spectra of the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25.. k is the Boltzmann constant. The ionic mobility, µ can be evaluated using Eq. (9):. μ=. σ dc ne. (9). The values of ωp, K, n and µ at room temperature studied for Mg0.5+x/2Si2-xAlx(PO4)3 compounds are presented in Table 3. The values of ωp, K, n and µ increase with the increase in x. This means that the rise in conductivity in the samples can be attributed to the extra Mg2+ interstitial ion which rises in ionic mobility as well as density of mobile ions [22–24]. Fig. 7 depicts the dielectric constant (ε’) versus log f for different x value of Mg0.5+x/2Si2-xAlx(PO4)3 samples. At low frequency region, the value of ε’ increases with the increase of x. This is due to the contribution of charge carrier accumulation at the interface of the sample and electrode [19–22]. This ε’ value is greater than the value in parent compound, Mg0.5Si2(PO4)3 as reported in reference [4]. It is proving that, the substitutions of Al3+ at the Si4+ lattice site (Si4+ ↔ Al3+ + 1/2Mg2+) affected the number of charge carrier in the sample. Fig. 8 shows the graph of dielectric loss (ε’’) of Mg0.5+x/2Si2-xAlx(PO4)3 as a function of log f at different value of. x. The ε’’ values also increase with the increase of x at low frequency region. It’s because, when the x value increases, the large amount of Mg2+ interstitial ions is created. The increase of Mg2+ interstitial ions results in high electrical energy loss due to the migration of ion to the surface of the sample which increases the value of ε’’ [22–25]. Fig. 9 presents the plot of frequency dependence of tan δ = ε’’/ ε’ at different x. The plot shows a peaking behavior for all x. As the x increases, the tan δ peaks are shifted toward higher frequency. The angular frequency ω (ω = 2π fmax) which. Table 3 Value of ωp, K, n and µ at room temperatures for Mg0.5+x/2Si2-xAlx(PO4)3 samples. Sample. ωp (Hz). K (S cm−1 K Hz−1). n × 1023 (cm−3). µ (cm2 V−1 s−1). x = 0.10 x = 0.15 x = 0.20 x = 0.25. 2.69 × 106 3.39 × 106 4.27 × 106 2.27 × 107. 4.11 × 10−10 7.48 × 10−10 7.60 × 10−10 7.97 × 10−10. 1.54 2.80 2.84 7.39. 1.48 × 10−10 1.87 × 10−10 2.35 × 10−10 2.35 × 10−09. Fig. 7. Plot of dielectric constant (ε’) as a function of log f of the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25..

(7) Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. Fig. 8. Plot of dielectric loss (ε’’) as a function of log f for the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25.. corresponds to maximum tan δ gives the relaxation times τ, from the relation [24,25].. ω maxτ = 1. (10). The relaxation times, τ is inversely proportional to jumping probability P which is expressed as [24,25]:. τ=. 1 P 2. (11). The τ for the samples with x = 0.10, 0.15, 0.20 and 0.25 are 1.71 × 103, 2.15 × 103, 4.28 × 103 and 4.28 × 104 Hz respectively. The results demonstrate that the ions in the sample x = 0.25 had the highest jumping probability. This value is higher compared to the τ value in parent compound, Mg0.5Si2(PO4)3 (3.8 × 104 Hz) as reported in reference [4]. Its. 445. Fig. 10. Linear sweep voltammogram of the Mg0.5+x/2Si2-xAlx(PO4)3 samples with x = 0.25 with a sweep rate of 50 mV s−1.. demostrated extra Mg2+ interstitial ion affected the jumping probability of ions in the sample. Linear sweep voltammetry was employed in this work to examine the decomposition voltage of the Mg0.5+x/2Si2-xAlx(PO4)3 electrolyte samples. The linear sweep voltammogram of the Mg0.5+x/2Si2-xAlx(PO4)3 sample with x = 0.25, which is the highest conducting compound is shown in Fig. 10. The value of voltage stability window of the magnesium electrolyte is found to be 2.51 V. This value is acceptable in magnesium battery system since the standard electrode potential between magnesium metal is less than 2.37 V [26]. Meanwhile Fig. 11 shows the plot of current vs. time for Mg/Mg0.625Si1.75Al0.25(PO4)3/Mg cell used for the magnesium transference number determination. Under a dc polarization of 0.27 V, the current in the both cells exhibits only a small decay with time. The initial and final steady current for the. Fig. 9. Frequency dependence of tan δ for the Mg0.5+x/2Si2-xAlx(PO4)3 samples with (a) x = 0.10, (b) x = 0.15, (c) x = 0.20 and (d) x = 0.25..

(8) 446. Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447. Fig. 11. Plot of current vs. time for Mg0.625Si1.75Al0.25(PO4)3 compound.. Mg/Mg0.625Si1.75Al0.25(PO4)3/Mg cell are Io = 4.87 × 10−6 A and Iss = 4.65 × 10−6 A respectively. The impedance responses of the cells prior to and after polarization for the Mg/ Mg 0.625 Si 1.75 Al 0.25 (PO 4 ) 3 /Mg cell are R o = 20,000 Ω and Rss = 29,000 Ω respectively. The value magnesium transfer number for Mg0.625Si1.75Al0.25(PO4)3 compound is 0.82 and confirmed the prepared compound was ionic. 4. Conclusion The effects of Mg2+ interstitial ion on the properties of Mg0.5+x/2Si2-xAlx(PO4)3 ceramic electrolytes were studied. The structure of the parent compound was affected by substitution of Al3+ and the increase of the Mg2+ interstitial ion. Meanwhile, the conductivity study on room temperature showed an increasing pattern up to 1.54 × 10−4 S cm−1. The conductivity parameters such as hopping frequencies, charge carrier concentration and mobile ion concentration proved that the increase in conductivity with x was due to the increase of the Mg2+ interstitial ion. The Mg0.625Si1.75Al0.25(PO4)3 sample exhibited a stable voltage window in voltage range of 2.51 V at ambient temperature. The value of magnesium transference number for the Mg0.625Si1.75Al0.25(PO4)3 sample was confirmed that the compound was ionic. Acknowledgement The authors would like to extend their gratitude toward the University of Malaya and Ministry of Education for funding this work through the Fundamental Research Grant Scheme (project no: FP006-2013B), University of Malaya Research. Grant (project no: RP013A-13AFR), and Postgraduate Research Grant (project no: PG032- 2015A). References [1] L. Dongping, X. Terrence, S. Partha, M.K. Datta, M.L. Gordin, A. Manivannan, et al., J. Electrochem. Soc. 160 (2) (2013) A351–A355. [2] N. Anuar, S.B.R.S. Adnan, N.S. Mohamed, Ceram. Int. 40 (2014) 13719–13727. [3] E. Levi, M. Levi, O. Chasid, D. Aurbach, J. Electroceram. 22 (2009) 13–19. [4] Z.A. Halim, S.B.R.S. Adnan, N.S. Mohamed, Ceram. Int. 42 (2016) 4452–4461. [5] Z. Khakpour, Electrochim. Acta 196 (2016) 337–347. [6] M. Illbeigi, A. Fazlali, M. Kazazi, A.H. Mohammadi, Solid State Ionics 289 (2016) 180–187. [7] S.B.R.S. Adnan, F.M. Salleh, N.S. Mohamed, Ceram. Int. 42 (15) (2016) 17941–17945. [8] S.B.R.S. Adnan, N.S. Mohamed, Ceram. Int. 40 (2014) 6373–6379. [9] T. Rahman, M. Vargas, C.V. Rama, J. Alloys Compd. 617 (2014) 547–562. [10] N.K. Anuar, S.B.R.S. Adnan, M.H. Jaafar, N.S. Mohamed, Ionics 22 (2016) 1125–1133. [11] P.G. Bruce, J. Evans, C.A. Vincent, Solid State Ionics 28–30 (1998) 918–922. [12] X. Wu, Z. Wen, X. Xu, X. Wang, J. Lin, J Nucl Mater 392 (2009) 471–475. [13] F. Wang, Y. Han, C.S. Lim, Y. Lu, J. Wang, J. Xu, et al., Nature 463 (2010) 1061–1065. [14] C. Xu, J. Tamaki, N. Miura, N. Yamazoe, Sens. Actuators B Chem. 3 (1991) 147–155. [15] R. Norhaniza, R. Subban, N.S. Mohamed, J. Mater. Sci. 46 (2011) 7815–7821. [16] C. Mariappan, G. Govindaraj, Solid state ionics 176 (2005) 1311–1318. [17] E. Traversa, H. Aono, Y. Sadaoka, L. Montanaro, Sens. Actuators B Chem. 65 (2000) 204–208. [18] A. Orliukas, A. Dindune, Z. Kanepe, J. Ronis, B. Bagdonas, A. Kežionis, Electrochim. Acta 51 (2006) 6194–6198. [19] D. Almond, G. Duncan, A. West, Solid State Ionics 8 (1983) 159–164..

(9) Z.A. Halim et al. / Journal of Magnesium and Alloys 5 (2017) 439–447 [20] R. Sobiestianskas, A. Dindune, Z. Kanepe, J. Ronis, A. Kežionis, E. Kazakevičius, et al., Materials Sci and Eng: B 76 (2000) 184–192. [21] M. Prabu, S. Selvasekarapandian, A. Kulkarni, G. Hirankumar, A. Sakunthala, Ionics 16 (2010) 317–321. [22] S.B.R.S. Adnan, N.S. Mohamed, Materials Research Innovations 16 (2012) 281–285. [23] N. Hegab, A. Bekheet, M. Afifi, L. Wahaba, H. Shehata, Journal Ovonic Research 3 (2007) 71–82.. 447. [24] M. Vijayakumar, G. Hirankumar, M. Bhuvaneswari, S. Selvasekarapandian, J. Power Sources 117 (2003) 143–147. [25] S.B.R.S. Adnan, N.S. Mohamed, International Journal of Electrochemical Science, International Journal of Electrochemical Science 7 (2012) 9844–9858. [26] R. Mohtadi, F. Mizuno, Beilstein Journal of Nanotechnology 5 (2014) 1291–1311..

(10)